Interconversion between ladder-type octanuclear and linear tetranuclear copper(i) complexes supported by tetraphosphine ligands
Takemura, Yukie; Nakajima, Takayuki; Tanase, Tomoaki; Dalton Transactions  (2009) 10231–10243; doi:10.1039/b909252h

data_7002839
_publ_section_title
;
 Interconversion between ladder-type octanuclear and linear
 tetranuclear copper(i) complexes supported by tetraphosphine ligands
;
_journal_issue                   46
_journal_name_full               'Dalton Transactions'
_journal_page_first              10231
_journal_page_last               10243
_journal_paper_doi               10.1039/b909252h
_journal_year                    2009
_chemical_formula_moiety         'C89.50 H106.50 Br4.80 Cu4 O5.75 P8 S5.75 '
_chemical_formula_sum            'C89.5 H106.5 Br4.8 Cu4 O5.75 P8 S5.75'
_chemical_formula_weight         2344.18
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_audit_creation_date             2009-08-05
_audit_creation_method           'by CrystalStructure 3.8'
_cell_angle_alpha                90.0000
_cell_angle_beta                 90.3600(8)
_cell_angle_gamma                90.0000
_cell_formula_units_Z            4
_cell_length_a                   15.5897(8)
_cell_length_b                   20.9612(9)
_cell_length_c                   33.0596(13)
_cell_measurement_reflns_used    18993
_cell_measurement_temperature    153(2)
_cell_measurement_theta_max      27.5
_cell_measurement_theta_min      3.0
_cell_volume                     10803.0(8)
_computing_cell_refinement       CrystalClear
_computing_data_collection       CrystalClear
_computing_data_reduction        CrystalStructure
_computing_molecular_graphics    ORTEP-II
_computing_publication_material  'CrystalStructure 3.8'
_computing_structure_refinement  SHELXL
_computing_structure_solution    SIR92
_diffrn_detector_area_resol_mean 7.31
_diffrn_measured_fraction_theta_full 0.658
_diffrn_measured_fraction_theta_max 0.659
_diffrn_measurement_device_type  'Rigaku Mercury'
_diffrn_measurement_method       \w
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71070
_diffrn_reflns_av_R_equivalents  0.043
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       42
_diffrn_reflns_limit_l_min       -42
_diffrn_reflns_number            64323
_diffrn_reflns_theta_full        27.50
_diffrn_reflns_theta_max         27.48
_exptl_absorpt_coefficient_mu    2.832
_exptl_absorpt_correction_T_max  0.428
_exptl_absorpt_correction_T_min  0.360
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Jacobson, R. (1998) Private communication'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.441
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             4742.00
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.35
_exptl_crystal_size_min          0.30
_refine_diff_density_max         2.35
_refine_diff_density_min         -1.98
_refine_ls_extinction_coef       none
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.390
_refine_ls_hydrogen_treatment    refall
_refine_ls_number_parameters     1111
_refine_ls_number_reflns         22846
_refine_ls_R_factor_gt           0.1008
_refine_ls_shift/su_max          0.0100
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w = 1/[\s^2^(Fo^2^)+(0.2130P)^2^+109.7027P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.2897
_reflns_number_gt                16012
_reflns_number_total             22846
_reflns_threshold_expression     F^2^>2.0\s(F^2^)
_cod_data_source_file            b909252h.txt
_cod_data_source_block           '_compound3b-revised'
_cod_original_formula_sum        'C89.50 H106.50 Br4.80 Cu4 O5.75 P8 S5.75 '
_cod_database_code               7002839